IOSR Journal of Applied Physics (IOSR-JAP) e-ISSN: 2278-4861. Volume 5, Issue 5 (Jan. 2014), PP 26-30 www.iosrjournals.org
Half-metallic-ferrimagnetic Sr2CrWO6 and Sr2FeReO6 materials for room temperature spintronics: Linear muffin-tin orbital studies M. Musa Saad H.-E., I. B. I. Tomsah, and A. Fiasal Elhag Department of Physics, College of Science, Qassim University, Buraidah 51452, Kingdom of Saudi Arabia
Abstract: Complex perovskite-like materials which include magnetic transition elements have relevance due to the technological perspectives in the spintronics industry. In this work, we report the studies of the electronic and magnetic characterizations of Sr2CrWO6 and Sr2FeReO6 as spintronics materials at room temperature by using the linearized muffin-tin orbitals (LMTO) method through the atomic-sphere approximation (ASA) within the local spin density approximation (LSDA). The interchange-correlation potential was included through the LSDA+U technique. The band structure results at room-temperature predict half-metallic ferrimagnetic ground state for Sr2CrWO6 and Sr2FeReO6 with total magnetic moment of 1.878 μB and 3.184 μB per formula unit, respectively, agreement with the previous theoretical and experimental results. Keywords: Complex perovskite; LMTO-ASA method; Half-metallic.
Complex perovskite oxides have the general chemical formula of A2BB'O6, crystalline in the rock-salt (Na+Cl–) structure with alternate perovskites ABO3 and AB'O3 along three crystallographical axes . The corners of each perovskite unit cell are in turn occupied by different transition-metals B and B', have the mixed valence state (BB')8+,with oxygen atoms located in between, forming alternate BO 6 and B'O6 octahedra [1-2]. The large alkaline-earth metal A2+ occupied the body-centered site with 12-fold oxygen coordination in each unit cell . The long-range superexchange interactions between magnetic ions in complex perovskite A2BB'O6 are in the form (– B – O – B' –) instead of double-exchange (– B – O – B –) in single perovskite ABO3 , . Materials with high spin-polarization of the conducting charge carriers, the current, have attracted a great deal of attention owing to their technological applications in spin-electronics (spintronics) , in magnetotransport devices, as well as their rich and challenging physical properties [1-6]. In particular, an ideal material with 100% spin-polarization is described as half-metal . Such materials can be found in several materials classes as in; magnetite Fe3O4 , CrO2 , LaMnO3 , Heusler alloy Co2(Cr1-xFex)Al , , as well as, in the group of complex perovskites ,[4-5]. Complex perovskites are of special attention, since within this group half-metals with above room-temperature (RT) transition temperatures are found, such as in A2FeMoO6 (A = Ca, Sr, Ba) [13-14] and Sr2CrMoO6 ,. Ordered complex perovskites Sr2FeMoO6, Sr2FeReO6, Sr2CrWO6, etc., are among the very few materials that allow electrons of one spin direction to move through them as though they were passing through a normal metal, while blocking electrons of the opposite spin. Materials that behave this way at RT are even more exotic, so their conduction bands have fully spinpolarized . Sr2FeReO6, Sr2CrWO6 complex perovskites, in particular, have attracted more attention due to their fairly high transition temperature from a paramagnetic to ferrimagnetic state, which makes them and their family of materials candidates for future spintronics applications.
In the present work we report systematic studies on the Cr/Fe (3d) and W/Re (5d) orbitals contributions to the electronic and magnetic structures of two close relative members of strontium complex perovskite oxides Sr2CrWO6 and Sr2FeReO6. Where, W and Re are neighboring 5d transition-metal elements in the periodic table with the ordinary electronic configurations of [Xe] 4f14 5dn 6s2, where n = 4 for W (Z = 74) or n = 5 for Re (Z = 75), where [Xe] denotes the configurations of the Nobel-gas Xenon core. For chromium and iron Cr/Fe (3d), Cr has an odd electron configuration of [Ar] 4s1 3d5 owing to the lower energy of the high spin configuration, not [Ar] 4s2 3d4 as it might expect, where a half-filled d sub-level is more energetically favorable than a half-filled s sub-level, so one of the 4s electrons is promoted to a 3d orbital. On the other hand, iron (Fe) has an ordinary electron configuration of [Ar] 4s2 3d6. Cr and Fe exhibit a wide range of possible oxidation states, where the +3 state is more stable energies [16-18]. Accordingly, the valence configurations of transition-metal ions in Sr2CrWO6 are; Cr3+ (3d3) and W5+ (5d1) in the high spin state with valence spin magnetic moments of S = 3/2 and S = 1/2 according to Hund's rule, respectively. Consequently, the theoretical total magnetic moment is 2.0 μB per formula unit cell for the ferrimagnetic ground state. In Sr 2FeReO6, Fe3+ (3d5) in the high spin state with S www.iosrjournals.org
26 | Page
Half-metallic-ferrimagnetic Sr2CrWO6 and Sr2FeReO6 materials for room temperature spintronics: = 5/2 and Re5+ (5d2) is highly ionized with valence spin magnetic moment of S = 1. As a result, the total magnetic moment for the ferrimagnetic ground state is 3.0 μB per Sr2FeReO6. For cubic Sr2CrWO6 and Sr2FeReO6 complex perovskites with space group Fm-3m (No. 225), we used the experimental lattice constants of a = 7.890 Å from (Ref. 19) and a = 7.832 Å from (Ref. 1), respectively, closed to the theoretical values calculated using SPuDS  7.880 Å and 7.886 Å, correspondingly. The magnetic structure in complex perovskites can be assigned to the AFM superexchange interactions between two very different transition magnetic ions ,, such as Cr/Fe (3d) and W/Re (5d), in this work, via intermediated O2ions (Cr/Fe – O – W/Re). In addition to, the naturally small magnetic moment at W/Re (5d) is believed to be not intrinsic but is induced by the strong magnetic ions Cr/Fe (3d).
The first-principles linear muffin-tin orbital (LMTO) method with atomic-sphere approximation (ASA) has been employed to perform self-consistent band structure calculations within the local spin density approximation (LSDA). In LMTO-ASA, which is similar to the multiple-scattering Korringa-Kohn-Rostoker (KKR) method  , the potential is approximated by a muffin tin potential, i.e., it is spherically symmetric around the atomic sites and constant in the interstitial volume. Moreover, ASA takes the one-electron potential and charge density to be spherically symmetric inside space-filling Wigner-Seitz (WS) spheres whose overlap is neglected, the interstitial volume, now integrating to zero . The von Barth–Hedin parameterization for exchange-correlation potential is used in the calculations , . The Hartree potential is expanded in term of spherical harmonic up to 6, therefore, Sr (5s 4p 4d), Cr/Fe (4s 4p 3d), Mo (5s 5p 4d), W (6s 6p 5d) and O (2s 2p) LMTOs were input as valence states, while Sr (4s), Cr/Fe (3p), Mo (4s 4p), W (5p 4f) fixed as semicore states in the unit cells. It has been established that the structures are close enough, that no empty sphere (ES) is needed to introduce the unit cells . The numbers of divisions along a reciprocal lattice vector which will set up the mesh for integrating valence state are selected as (6 × 6 × 6). Special k points of 50 in the irreducible Brillouin zone (IBZ) were used in band structure and density of states calculations. A single kappa LMTOs basis set is expanded in spherical harmonic up to the angular momentum l max = 6, was used for the valence-band charge densities and potential inside the non-overlapping muffin-tin spheres . The interchange-correlation potential was included through the LSDA+U technique, where the on-site Coulomb energy (U) has been in used. The correlation parameters, Coulomb energy (U) and Hund's rule exchange (J), were utilized for strongly correlated 3d and weakly 5d electrons in the calculations. The Hubbard parameters (U = 4.0 eV, J = 0.98 eV) are used for Cr/Fe (3d) states (Refs. 1.0 and 17), even as (U = 1 eV, J = 0.96 eV) are used for W/Re (5d) states (Refs. 1 and 17). The resolving of spin up and down in total and partial densities of states for Sr2CrWO6 and Sr2FeReO6 were calculated and obtained from the LSDA+U calculations.
Results and Discussion
Fig. 1 illustrates the total densities of states (TDOSs) of Sr2CrWO6 and Sr2FeReO6 from band structure LSDA+U calculations. The obtained results of Sr2CrWO6 and Sr2FeReO6 are in agreement with previous LSDA+U calculations ,,. In spin-up TDOSs, there are energy gaps of about 1.33 eV in Sr2CrWO6 and 2.18 eV in Sr2FeReO6 between the occupied Cr/Fe (3d) and unoccupied W/Re (5d) partial bands. Since the energy gap in the spin-up produces from the antiferromagnetic coupling between Cr/Fe (3d) and W/Re (5d) states, as shown in Fig. 2, this situation emerges as peaks of 3d and 5d bands polarized antiferromagnetically demonstrate the Cr/Fe (3d) ↑ and W/Re (5d) ↓ form. Therefore, the spin-up electrons are insulating while the spin-down electrons are metallic, resulting in full (100%) spin-polarized of the conduction electrons at EF. For that reason, Sr2CrWO6 and Sr2FeReO6 materials allow electrons of spin-down direction to move through them as though they were passing through a metal, while blocking electrons of the spin-up.
Fig. 1. Total density of states (TDOS) for (a) Sr2CrWO6, and (b) Sr2FeReO6 www.iosrjournals.org
27 | Page
Half-metallic-ferrimagnetic Sr2CrWO6 and Sr2FeReO6 materials for room temperature spintronics:
Fig. 2. Total and partial densities of states for (a) Sr2CrWO6, and (b) Sr2FeReO6 As seen in Fig. 2, the conduction bands in spin-down orientation is attributed mainly to the contributions of W (5d) and Re (5d) ions with tiny contributions of Cr (3d) and Fe (3d), correspondingly. Compare the TDOSs with PDOSs, the level distributions in of Sr2CrWO6 and Sr2FeReO6 are overall very similar, except a peak between 1.0 eV and 3.0 eV, above EF, is higher in Sr2FeReO6 than in Sr2CrWO6. This dissimilarity, as seen in Fig. 2, due to the extra electron in Re (5d2) than in W (5d1). In order to understand in some more detail the origin of the electronic and magnetic characters of Sr2CrWO6 and Sr2FeReO6, we critically examine the partial electronic density of states (PDOS) of these systems. The basic critical ingredients in the TDOS are the d states of the Cr/Fe and W/Re atoms, which in turn are split into t2g and eg states by the octahedral crystal field (OCF) produced by the oxygen octahedra. The t2g states having lower energy and place for three electrons per spin channel, whereas the eg states are higher in energy and have places for two electrons per spin channel. Furthermore, due to the exchange splitting, t2g bands degenerate into double orbitals (dxz and dyz) and one singlet orbital (dxy), while eg bands degenerate into two singlet orbitals (dx2–y2 and dz2), as seen in Fig. 3, which show the partial densities of states of t2g, eg and 2p orbitals in Sr2CrWO6 and Sr2FeReO6. From the PDOS in Fig.3 (a), the threefold degenerate Cr t 2g states of the spin-up channel are filled Cr3+ 3 3 (3d : t2g ↑); consequently the dxy↑, dxz↑ and dyz↑ orbitals are at the energy range, about –7 eV ~ –1.5 eV in the valance bands. Therefore, the EF ends up in the CF gap of ∆o ≈ 1.5 eV between Cr t2g and eg states. A similar situation is observed in the half-metallic close-relative Sr2FeReO6 , . Due to the antiferromagnetic coupling in Cr (3d) – W (5d), it is the spin-down channel in W (5d) which is the occupied one, and it contains one electron in t2g states W5+ (5d1: t2g1↓). This means that the W (5d) t2g spin-down states are only filled to about one-two, resulting in high density of states of d xy and dyz at the EF in spin-down channel. In addition to, due to hybridization between states in Sr2CrWO6, Cr t2g↓ states achieved small occupation, while W (5d) states in the spin-up channel are essentially empty; hybridization with Cr t2g↑ states results nevertheless in a finite, small occupation above EF.
Fig. 3. Partial densities of states of t2g, eg and 2p orbitals in (a) Sr2CrWO6, and (b) Sr2FeReO6 www.iosrjournals.org
28 | Page
Half-metallic-ferrimagnetic Sr2CrWO6 and Sr2FeReO6 materials for room temperature spintronics: On the other hand, from the PDOS in Fig.3 (b), the Fe t2g and eg states are full-filled in the spin-up orientation; Fe3+ (3d5: t2g3↑ eg2↑) in the high spin state; the electronic configuration can be set of orbitals as (dxy↑)1, (dxz↑ and dyz↑)2, (dx2 –y2)1 and (dz2)1 extend from –8.0 eV to -2.0 eV in the valence bands. The exchange splitting is about 7.5 eV, larger than the CF splitting, ∆o ≈ 2.25 eV, resulting in the high-spin of Fe (3d) states. At the same time, spin-down channel in Re (5d) which is the occupied one, and it contains two electrons in t2g states Re5+ (5d2: t2g2↓). Therefore, the Re t2g spin-down states are only filled to about two-three, emerged as a high spin-down DOS of dxy and dyz at EF. Inversely, neither Fe t2g↓ nor Re (5d)↑ states have contributed to the bands around EF, while the O (2p) bands are at a much lower energy from –9.0 to –2.0 eV. Finally, the magnetic structure in Sr2CrWO6 and Sr2FeReO6 complex perovskites can be assigned to the antiferromagnetic superexchange interactions between Cr/Fe (3d) and W/Re (5d) via intermediated oxygen atoms in the 180o long-chain Cr (3d-t2g↑) – O (2pπ) – W (5d-t2g↓) and Fe (3d-t2g↑) – O (2pπ) – Re (5d-t2g↓), correspondingly. The calculated spin magnetic moments from LSDA+U for Sr2CrWO6 are; 2.919 μB for Cr, – 1.044 μB for W with a total magnetic moment of 1.878 μB, which is 94% agreement with the later LSDA+U result, 2.01 μB , . For Sr2FeReO6, 4.578 μB for Fe, –1.344 μB for Re, and the total magnetic moment found to be 3.184 μB, also, agree to the LSDA+U result, 3.06 μB . The bands scheme for both compounds are illustrated in Fig. 4, the results can be resumed by means the simple model describes the effect of filling t2g and eg orbitals in 3d and 5d bands for spin-up and spin-down configurations.
eg0 W t2g1
Fe t2g3 Cr t2g3
Fig. 4. Representation of the electronic density of spin-up (↑) and spin-down (↓) states in 100% electronic spinpolarized half metal in the Sr2CrWO6 and Sr2FeReO6 materials. The quantity of filling signifies the effect of t2g and eg orbitals in 3d and 5d bands per unit volume and per unit energy E. EF is the Fermi energy.
We have comparatively studied the electronic and magnetic characterizations of complex perovskites Sr2CrWO6 and Sr2FeReO6 by using the linearized muffin- tin orbitals through the atomic-sphere approximation method within the local spin density approximation, including the interchange-correlation potential through the LSDA+U technique. The band structure results demonstrated half-metallic ferrimagnetic ground state for Sr2CrWO6 and Sr2FeReO6 with total magnetic moment of 1.878 μB and 3.184 μB per formula unit, respectively, in exact agreement with the theoretical and experimental results. The obtained HM-FiM feature in complex perovskites Sr2CrWO6 and Sr2FeReO6 makes these materials suitable for many applications. It established that they have a high degree of electronic spin-polarization which means that they will have the potential spin transport electronics (spintronics), where spin currents are utilized as well as charge currents.
Acknowledgments The authors gratefully acknowledge financial support from the Deanship of Scientific Research, Qassim University in KSA, under the Grant Name Research-backed research priorities for the year 1432 – 1433 AH, and Project Number 1622.
29 | Page
Half-metallic-ferrimagnetic Sr2CrWO6 and Sr2FeReO6 materials for room temperature spintronics: References
                       
Horng-Tay Jeng, and G. Y. Guo, Phys. Rev. B 67, 094438, (2003) 1 – 7. L. Brey, M. J. Calderón, S. Das Sarma, and F. Guinea, Phys. Rev. B 74, 094429 (2006) 1-7. A. H. Habib, A. Saleem,C. V. Tomya, D. Bahadur, J. Appl. Phys. 97, 10A906 (2005) 1- 4. J. Cheng and Z. Q. Yang, Phys. Stat. sol. (b) 243, No. 6 (2006) 1151 – 1158. I. V. Solovyev, Phys. Rev. B 65, 144446 (2002) 1-17. Tapas Kumar Mandal, Claudia Felser, Martha Greenblatt, and Jurgen Kubler, Phys. Rev. B 78, 134431 (2008) 1 – 8. G. Vaitheeswaran, V. Kanchana, and A.Delin, Appl. Phys. Letts. 86, 032513 (2005) 1–3. S. Jain, A. O. Adeyeye, and C. B. Boothroyd, J. Appl. Phys. 97, 093713, (2005). Joonghoe Dho, Sanghoon Ki, A. F. Gubkin, J. M. S. Park, and E. A. Sherstobitova, Solid State Commun. 150, (2010) 80 – 90. L. C. Moreno, J. S. Valencia, D. A. Landinez Tellez, J. Arbey Rodriguez M., M. L. Martinez, J. Roa-Rojas, and F. Fajardo, J. Magnets. Magnet. Mater. 320, (2008) 19-21. Koichiro Inomata, Naomichi Ikeda, Nobuki Tezuka, Ryogo Goto, Satoshi Sugimoto, Marek Wojcik, and Eva Jedryka, Sci. Technol. Adv. Mater. 9, 014101, (2008). Yoshio Miura, Kazutaka Nagao, and Masafumi Shirai, Phys. Rev. B 69, 144413 (2004)1-7. C. M. Bonilla, D. A. Landinez, J. Arbey, E. Vera Lopez and J. Roa-Rojas, Physica B 398, (2007) 208 – 211. Akira Isayama, Shogo Kadota, Hideomi Yui, and Takao Sasagawa, Mater. Scien. Engin.: B 173, (2010) 44 - 46. Q F Li, X F Zhu, and L F Chen, J. Phys.: Condens. Matter 20, 255230 (2008) 1 – 8. M. El-Hagary, J. Alloys and Compounds 502, 2, (2010) 376 – 381. Hua Wu, Phys. Rev. B 64, 125126, (2001). J. B. Philipp, P. Majewski, L. Alff, R. Gross, T. Graf, M. S. Brandt, J. Simon, T. Walther, W. Mader, D. Topwal, and D. D. Sarma, Phys. Rev. B 68, 144431 (2003). J. B. Philipp, D. Reisinger, M. Schonecke, A. Marx, A. Erb, L. Alff, R. Gross, and J. Klein, Appl. Phys. Letts. 79, 3654 (2001) 1 3. M. Zwierzycki and O. K. Andersen, Acta Physica Polonica A, 1, V. 115 (2009). G. Vaitheeswaran, V. Kanchana, and A.Delin, Appl. Phys. Letts. 86, 032513 (2005) 1–3. G. Vaitheeswaran, V. Kanchana and A.Delin, J. Phys.: Confer. Ser. 29 (2006) 50 - 53. Yan Zhang, Vincent Ji, Physica B: Condens. Matter 407, 5, (2012) 912 – 917. T. S. Chan, R. S. Liu, G. Y. Guo, S. F. Hu, J. G. Lin, J. –F. Lee, L. –Y. Jang, C. –R. Chang and C. Y. Huang, Solid State Commun. 131 (2004) 531 - 535.
30 | Page